Successfully reported this slideshow.
You’ve unlocked unlimited downloads on SlideShare!
“NON WOVEN ”
Omkar S. Parmaj
Research scholar in Institute of chemical technology Mumbai
A nonwoven is a textile structure produced by the bonding or interlocking of
fibres, or both, accomplished by mechanical, chemical, thermal or solvent
means and combinations thereof.
It is generally done in one continuous process directly from the raw material
to the finished fabric.
All nonwoven processes can be divided into two stages, the preparation of
the fibres into a form suitable for bonding and the bonding process itself.
The great advantages in non-woven fabrics is the speed with which the final
fabric is produced.
All yarn preparation steps are eliminated, and the fabric production itself is
faster than conventional methods.
To produce 500,000 meters of woven sheeting requires 2 months of yarn
preparation, 3 months of weaving on 50 looms and 1 month for finishing and
Non-woven fabric can deliver the same quantity of sheeting within 2 months
NATURAL FIBRES AND REGENERATED MAN-MADE FIBRES
WOVEN FABRIC PRODUCTION METHOD:-
In the woven fabric production method, the following steps are carried out
Fibre Yarn formation Fabric formation
For convertion of fibres to fabric production first fibre is converted into yarn form with help of
spinning and then the yarn is converted into the fabric form with the help of weaving loom.
NON WOVEN FABRIC PRODUCTION METHOD:-
In the non woven fabric production method, requires only two stages
Fibres Non woven fabric
The non woven fabric production eliminates the yarn production process and makes the fabric directly
from fibres. The fibre is directly converted in to the interlacing of fibres with chemical or mechanical
There are normally two steps for making non-woven products.
1. Web formation; and
2. Bonding systems.
Web formation Bonding system with chemical or mechanical means
The mass per unit area of card web is normally too low to
be used directly in a nonwoven.
three cards raised slightly above the floor to allow
a long conveyor lattice to pass underneath.
The webs from each card fall onto the lattice forming a batt
with three times the mass per unit area.
The card webs are turned through a right angle by a guide
at 45°, but the batt produced by this method is identical in
all respects to the previous method.
Since in parallel laying all the card webs are parallel to each
other (and to the batt), it follows that most of the fibres will
lie along the batt and very few across it.
A tensile test on a bonded parallel-laid material in the
machine direction will depend mainly on the fibre strength,
whereas in the cross direction it will depend more on the
When cross laying, the card (or cards) are placed at right angles
to the main conveyor just as in Fig.
but in this case the card web is traversed backwards and
forwards across the main conveyor, which itself is moving. The
result is a zig-zag.
Usually the conveyor B is moving only slowly so that many layers
of card web are built up, as shown in the diagram.
There are two major problems with cross layers; one is that they
tend to lay the batt heavier at the edges than in the middle.
However, this is not so because the cross-laying angle is
normally less than 10°, so that the great majority of fibres lie in
or near the cross direction.
Cross-laid fabrics are consequently very strong in the cross
direction and weak in the machine direction.
The air-laying method produces the final batt in one stage without first
making a lighter weight web.
Opened fibre from the opening/blending section is fed into the back of
hopper A, which delivers a uniform sheet of fibres to the feed rollers.
It is also capable of running at high production speeds but is similar to the
parallel-lay method in that the width of the final batt is the same as the
width of the air-laying machine, usually in the range of 3–4m.
The degree of fibre opening available in an air-lay machine varies from one
manufacturer to another, but in all cases it is very much lower than in a
The fibre is then taken by the toothed roller B, which is revolving at high
A strong air stream C dislodges the fibres from the surface of roller B and
carries them onto the permeable conveyor on which the batt is formed.
The wet-laid process is a development from papermaking that was undertaken because the
production speeds of papermaking are very high compared with textile production.
Textile fibres are cut very short by textile standards (6–20mm), but at the same time these
are very long in comparison with wood pulp, the usual raw material for paper.
It has been agreed that a material containing 50% textile fibre and 50% wood pulp is a
They are used widely in disposable products, for example in hospitals as drapes, gowns,
sometimes as sheets, as one-use filters, and as coverstock in disposable nappies.
The paper industry has attempted for many years to develop a dry paper process because
of the problems associated with the normal wet process, that is, the removal of very large
volumes of water by suction, by squeezing and finally by evaporation.
Now a dry process has been developed using wood pulp and either latex binders or
thermoplastic fibres or powders to bond the wood pulp together to replace hydrogen
bonding which is no longer possible.
Hence although the drylaid paper process cannot be regarded as a nonwoven process at
present, it is very likely that the process will be modified to accept textile fibres and will
become very important in nonwovens in the future. It is for this reason that it has been
Spun laying includes extrusion of the filaments from the polymer raw
material,drawing the filaments and laying them into a batt.
Spun laying starts with extrusion. Virtually all commercial machines use
thermoplastic polymers and melt extrusion.
The polymer chips are fed continuously to a screw extruder which delivers
the liquid polymer to a metering pump and thence to a bank of spinnerets,
or alternatively to a rectangular spinneret plate, each containing a very
large number of holes.
The liquid polymer pumped through each hole is cooled rapidly to the solid
state but some stretching or drawing in the liquid state will inevitably take
In spun laying the most common form of drawing the filaments to obtain
the correct modulus is air drawing, in which a high velocity air stream is
blown past the filaments moving down a long tube.
The process of melt blowing is another method of producing very fine fibres at high production rates
without the use of fine spinnerets.
polymer is melted and extruded in the normal way but through relatively large holes.
As the polymer leaves the extrusion holes it is hit by a high speed stream of hot air at or even above its
melting point, which breaks up the flow and stretches the many filaments until they are very fine.
At a later stage, cold air mixes with the hot and the polymer solidifies, Depending on the air velocity after
this point a certain amount of aerodynamic drawing may take place but this is by no means as satisfactory
as in spun laying and the fibres do not develop much tenacity.
The fine staple fibres produced in this way are collected into a batt on a permeable conveyor as in air laying.
In the bonded or laminated form the fabric can be used for breathable protective clothing in hospitals,
agriculture and industry, as battery separators, industrial wipes and clothing interlinings with good
TYPES OF CHEMICAL BONDING:-
Chemical bonding involves treating either the complete batt or alternatively isolated
portions of the batt with a bonding agent with the intention of sticking the fibres
As implied by the name, saturation bonding wets the whole batt with bonding agents, so
that all fibres are covered in a film of binder.
The action of the liquid greatly reduces the thickness of the batt and the thickness is
further reduced by the squeeze rollers which follow.
Because the air only penetrates the immediate surfaces of the nonwoven, drying is
confined to these areas and the central layers of the nonwoven remain wet The result is
that the liquid wicks from the wet areas to the dry ones, unfortunately carrying the
suspended binder particles with the water.
This is the cause of the problem known as binder migration; under adverse conditions
virtually all the binder can be found in the surface layers and the central layers contain no
binder at all, leaving them very weak.
Fortunately a number of ways have been found to control binder migration, several of
them being rather complicated.
It can be inferred above that one of the problems of saturation bonding is
that too much water is used.
This not only increases the cost of drying but also increases the risk of binder
The binder solution and a measured volume of air are passed continuously
through a driven turbine which beats the two components into a consistent
The foam is then delivered to the horizontal nip of the impregnating roller.
The foam delivery has to be traversed because the foam does not flow
easily; end plates, which cannot be shown in the cross-section diagram
prevent the foam from running out of the gap at the end of the rollers.
Foam application should only be thought of as an alternative method of
The properties and uses of the fabrics are identical.
Print bonding involves applying the same types of binder to the batt but the
Application is to limited areas and in a set pattern.
The binder does not penetrate well into the dry batt so the batt is first
saturated with water and then printed with either a printing roller or a rotary
The final properties of the fabric depend vitally on the printed/unprinted
area ratio, which could be changed significantly if the binder migrated
sideways from the printed area.
To prevent this the binder formulation must contain some thickener.
Print-bonded fabrics are much softer in feel and also much more flexible
owing to the strong effect of the free fibres in the unbonded areas.
Similar latex binders may also be applied by spraying,
using spray guns similar to those used in painting, which
may be either operated by compressed air or be airless.
On the first passage the spray penetrates about 5 mm
into the top surface, then the batt is turned over for a
spray application on the lower surface.
Each spray application reduces the thickness of the batt
slightly, but it is still left substantially lofty; the drying and
curing stage also causes some small dimensional
The final product is a thick, open and lofty fabric used
widely as the filling in quilted fabrics, for duvets, for
some upholstery and also for some types of filter media.
Thermal bonding is increasingly used at the expense of chemical bonding for a number of
reasons. Thermal bonding can be run at high speed, whereas the speed of chemical bonding is
limited by the drying and curing stage.
Thermal bonding can use three types of fibrous raw material, each of which may be suitable in
some applications but not in others.
THERMAL BONDING WITHOUT PRESSURE
THERMAL BONDING WITH SOME PRESSURE
THERMAL BONDING WITH HIGH PRESSURE
THERMAL BONDIING WITH POINT CONTACT
All the methods of bonding discussed so far have involved adhesion
between the fibres; hence they can be referred to collectively as
Needle punching is rely on frictional forces and fibre entanglements,
and are known collectively as mechanical bonding.
The batt or web is led between two stationary plates, the bed and
stripper plates, as shown in Fig. While between the plates the batt is
penetrated by a large number of needles, up to about 4000m-1 width
of the loom.
The needles are usually made triangular and have barbs cut into the
When the needles descend into the batt the barbs catch some fibres
and pull them through the other fibres.
When the needles return upwards, the loops of fibre formed on the
downstroke tend to remain in position, because they are released by
The idea of stitch bonding was developed almost exclusively in Czechoslovakia, in the former East Germany
and to some extent in Russia, though there was a brief development in Britain.
The machines have a number of variants which are best discussed separately; many possible variants have
been produced but only a limited number are discussed here for simplicity.
TYPES OF STITCH BONDING:-
BATT BONDED BY THREADS
STITCH BONDING WITHOUT THREADS
STITCH BONDING TO PRODUCE TO PILE FABRIC
BATT LOOPED THROUGH SUPPORTING STRUCTURE
LAID YARN SEWN TOGHTER WITH BINDING THREADS
Hydro- entangling by water jet is rely on frictional forces and fibre
entanglements, and are known collectively as water bonding.
Litter batt is used for Hydeo-entanglement.
As the name implies the process depends on jets of water working
at very high pressures through jet orifices with very small diameters
A very fine jet of this sort is liable to break up into droplets,
particularly if there is any turbulence in the water passing through
If droplets are formed the energy in the jet stream will still be
roughly the same, but it will spread over a much larger area of batt
so that the energy per unit area will be much less.
Consequently the design of the jet to avoid turbulence and to
produce a needle-like stream of water is critical.
The jets are arranged in banks and the batt is passed continuously
under the jets held up by a perforated screen which removes most
of the water.
AUTOTECH HOME FURNISHING
LEISURE AND TRAVEL TEXTILEAGRO TEXTILE
PERSONAL AND HEIGEN
g e cusick (ed.), Nonwoven Conference, Manchester, University of Manchester Institute of Science and
a newton and j e ford, ‘Production and properties of nonwoven fabrics’, Textile Progr., 1973 5(3) 1–93.
p j cotterill, ‘Production and properties of stitch-bonded fabrics’, Textile Progr., 1975 7(2) 101–135.
a t purdy, ‘Developments in non-woven fabrics’, Textile Progr., 1980 12(4) 1–97.
k pfliegel, ‘Nonwovens for use in the geotextile area’, Textile Institute Ind., 1981 19 178–181.
a krauter and p ehler, ‘Aspects of fibre to binder adhesion in nonwovens’, Textil Praxis Int., 1980, No.
10, 1206–1212; No. 11, 1325–1328.
anon, ‘Foam padder and foam production for the nonwoven industry’, Chemiefaser/Textilindustrie
(English edition), 1981 4, E.35–36 in English (pp. 336–338 in German).
g e cusick and a newton, (eds), ‘Nonwovens Conference’, Manchester, University of Manchester Institute
of Science and Technology, 1988.
g e cusick and k l ghandi, (eds), ‘Conference on nonwovens’, Huddersfield, University of Huddersfield,
a j rigby and s c anand, ‘Nonwovens in medical and healthcare products’, Tech. Textiles Int., 1996, Part
I, Sept. pp. 22–28 Part II, Oct. pp. 24–29.
Index 1999 Congress, Geneva, EDANA (European Disposables and Nonwovens Association), Brussels,